National Institute of Standards and Technology synchrotron radiation facilities for materials science.
Synchrotron Radiation Facilities A list of storage rings and free electron lasers used as synchrotron radiation sources by country. Armenia
A multidisciplinary field concerned with the generation and application of knowledge relating to the composition, structure, and processing of materials to their properties and uses. Laboratory of the National Institute of Standards and Technology National Institute of Standards and Technology, governmental agency within the U.S. Dept. of Commerce with the mission of "working with industry to develop and apply technology, measurements, and standards" in the national interest. , include beam stations at the National Synchrotron Light Source The National Synchrotron Light Source (NSLS) at Brookhaven National Laboratory (BNL) in Upton, New York is a national user research facility funded by the U.S. Department of Energy (DOE). at Brookhaven National Laboratory Brookhaven National Laboratory, scientific research center, at Upton (town of Brookhaven), Long Island, N.Y. It was founded in 1947 by Associated Universities, a management corporation sponsored by nine eastern U.S. universities. and at the Advanced Photon Source The Advanced Photon Source (APS) at Argonne National Laboratory is a national synchrotron-radiation light source research facility funded by the United States Department of Energy, Office of Science, Office of Basic Energy Sciences. at Argonne National Laboratory Argonne National Laboratory, research center, based in Argonne, Ill., 27 mi (43 km) SW of downtown Chicago, with other facilities at the Idaho National Engineering Laboratory, 50 mi (80 km) W of Idaho Falls, Idaho. Founded in 1946 by the U.S. . The emphasis is on materials characterization at the microstructural and at the atomic and molecular levels, where NIST (National Institute of Standards & Technology, Washington, DC, www.nist.gov) The standards-defining agency of the U.S. government, formerly the National Bureau of Standards. It is one of three agencies that fall under the Technology Administration (www.technology. scientists, and researchers from industry, universities and government laboratories perform state-of-the-art x-ray measurements on a broad range of materials.
Key words: ceramics; materials science materials science
Study of the properties of solid materials and how those properties are determined by the material's composition and structure, both macroscopic and microscopic. ; metallurgy; polymers; semiconductors; synchrotron synchrotron: see particle accelerator.
Cyclic particle accelerator in which the particle is confined to its orbit by a magnetic field. The strength of the magnetic field increases as the particle's momentum increases. radiation; x-ray instrumentation.
Synchrotron radiation sources provide intense beams of x rays for leading-edge research in a broad array of scientific disciplines. The National Institute of Standards and Technology (NIST) Materials Science and Engineering Laboratory (MSEL MSEL Materials Science and Engineering Laboratory
MSEL Milton S. Eisenhower Library (Johns Hopkins University)
MSEL Master Scenario Events List
MSEL Master of Studies in Environmental Law ) program to characterize materials by means of this powerful probe began in the early 1980s, with the design, construction and commissioning of a monochromatic monochromatic /mono·chro·mat·ic/ (-kro-mat´ik)
1. existing in or having only one color.
2. pertaining to or affected by monochromatic vision.
3. staining with only one dye at a time. x-ray topography (1) station (X23A3) at the National Synchrotron Light Source (NSLS NSLS North Suburban Library System
NSLS National Synchrotron Light Source ) at Brookhaven National Laboratory. The topography station, which was home to the only dedicated monochromatic topography instrument of its kind in the country, also included experimental facilities for hard x-ray microscopy (2) and parallel beam x-ray microradiography microradiography /mi·cro·ra·di·og·ra·phy/ (mi?kro-ra?de-og´rah-fe) radiography under conditions which permit subsequent microscopic examination or enlargement of the radiograph up to several hundred linear magnifications. . By 1989, an ultra-small-angle x-ray scattering (USAXS) instrument (3) had been added to X23A3, specifically for the purpose of enabling anomalous ultra-small-angle x-ray scattering. It was later used for a wide variety of USAXS measurements on ceramics (4), metals (5) , polymers (6) and biomaterials (7).
Today, the NIST/MSEL synchrotron radiation program includes the utilization and operation of three additional beam stations at the NSLS. X23A2 serves a large x-ray absorption fine structure X-ray absorption fine structure (XAFS) is a specific structure observed in X-ray absorption spectroscopy (XAS). By analyzing the XAFS, information can be acquired on the local structure and on the unoccupied electronic states. (XAFS XAFS X-Ray Absorption Fine Structure ), diffraction anomalous fine structure (DAFS (Direct Access File System) A high-performance file sharing protocol based on the VI memory-to-memory architecture. Designed for storage area networks (SANs), DAFS provides bulk data transfer directly between the application buffers of two machines without ), and x-ray spectroscopy x-ray spectroscopy
X-ray spectrometry. community. It provides stable scanning of monochromatic x rays in the energy range from 4.9 keV to over 30 keV. X24A, which is a shared beam station, provides incident x rays in the 1.7 keV to 6 keV energy range, and is used by NIST researchers for standingwave x-ray measurements. Finally, the U7A station, which is also a joint effort, utilizes x-ray photoemission spectroscopy Photoemission Spectroscopy (PES) also known as photoelectron spectroscopy, refers to energy measurement of electrons emitted from solids, gases or liquids by the photoelectric effect, in order to determine the binding energies of electrons in a substance. (XPS (1) See XML Paper Specification.
(2) A brand name for certain models of Inspiron laptops from Dell. ) and near-edge x-ray absorption fine structure (NEXAFS NEXAFS Near-Edge X-ray Absorption Fine Structure ) to study the structure and chemical nature of diverse materials from a surface and bulk perspective either in vacuum or under atmospheric reaction conditions. Taken together, these three NIST/MSEL beam lines at the NSLS provide continuously tunable x rays from 0.18 keV to over 30 keV, which covers spectroscopically nearly the entire periodic table.
Looking toward the future, NIST/MSEL became a partner in 1995 with the University of Illinois University of Illinois may refer to:
This paper is a highly selective review, by members of the current Materials Microstructure mi·cro·struc·ture
The structure of an organism or object as revealed through microscopic examination.
a structure on a microscopic scale, such as that of a metal or a cell Characterization Group, of the past two decades of research efforts of the scientists who built these facilities and currently are responsible for their operation. The emphasis is on the broad range of science performed by NIST researchers and others, enabled by facilities that were designed, constructed, commissioned and operated by NIST. Many additional contributions of colleagues and collaborators can be found in the references and acknowledgements at the end.
2. NIST programs at the National Synchrotron Light Source
2.1 Monochromatic Synchrotron X-Ray Topography
From 1984, until it was closed in 2000, X23A3 was a premier monochromatic x-ray topography facility. X-ray topography is a nondestructive non·de·struc·tive
Of, relating to, or being a process that does not result in damage to the material under investigation or testing.
non characterization technique for imaging, by means of x-ray diffraction, the micrometer-sized to centimeter-sized defect microstructure of crystals. The NIST Group's early research concentrated largely on crystal growth and crystal perfection as a function of processing. The power of the monochromatic topography instrument was the result of the early realization (8) that it is possible to design and build topographic optics to record images of the entire sample in a single exposure. While the first topography camera was built in the laboratory, similar principles were used in the design of the X23A3 instrument. Early studies included the observation of magnetic domains within single-crystal grains of pure nickel. The formation of domain walls near the crystal surface was also observed (Fig. 1). Later on, the excellent resolution of the instrument--of the order of 1.7 [micro]m--enabled detailed studies of bismuth-silicon-oxide (BSO BSO Bilateral salpingo-oophorectomy. Excision of both ovaries ). Three crystal slices from a single boule boule
Deliberative council in the city-states of ancient Greece. It existed in almost all constitutional city-states, especially from the late 6th century BC. In Athens the boule was created as an aristocratic body by Solon in 594 BC; later, under Cleisthenes, 500 members of BSO were examined, and the progression of microscopic strain as a function of growth was documented (9). Remarkably, all of the features that were recorded (Fig. 2) were growth striations that could be directly related to the growth habit of the crystal boule. Recent work has included topographic examination of biological crystals grown in space (10). One of the outstanding questions in protein crystal growth is the effect of gravity on the growth process. The crystallization Crystallization
The formation of a solid from a solution, melt, vapor, or a different solid phase. Crystallization from solution is an important industrial operation because of the large number of materials marketed as crystalline particles. of proteins can be strongly affected by gravity through sedimentation and convection. With the minimization of these processes, through growth in microgravity mi·cro·grav·i·ty
1. An environment in which there is very little net gravitational force, as of a free-falling object, an orbit, or interstellar space.
2. , will it become possible to produce better quality crystals? To answer this question, a comparison was made between ribonuclease Ribonuclease
A group of enzymes, widely distributed in nature, which catalyze hydrolysis of the internucleotide phosphodiester bonds in ribonucleic acid (RNA). crystals grown on the space shuttle and control crystals grown at the same time on Earth. A comparison of x-ray topographs recorded from Earth-grown and space-grown crystals is shown in Fig. 3. The space crystal has symmetry about the vertical and horizontal axes consistent with growth sectors. As the Bragg angle is changed, the four dark regions indicated migrate together toward or away from the center of the crystal, consistent with a central nucleation nu·cle·a·tion
1. The beginning of chemical or physical changes at discrete points in a system, such as the formation of crystals in a liquid.
2. The formation of cell nuclei. point followed by homogeneous growth. The microstructure of the Earth-grown crystal is less well defined, consistent with a higher defect density. The topography results were able to delineate some of the ways in which the minimization of gravity improves the quality of space-grown crystals.
2.2 Ultra-small-Angle X-Ray Scattering
The X23A3 beam line was also host to an ultra-small-angle x-ray scattering facility (3,11). This instrument offered high angular and wavelength resolution, large sample cross sectional area, accurate energy tuning, excellent signal-to-noise ratio The ratio of the power or volume (amplitude) of a signal to the amount of unwanted interference (the noise) that has mixed in with it. Measured in decibels, signal-to-noise ratio (SNR or S/N) measures the clarity of the signal in a circuit or a wired or wireless transmission channel. at ultra-small scattering vectors, and primary calibration of the absolute intensity. The scattering vector range available with this instrument served to bridge the gap between visible light scattering and standard x-ray scattering instruments. Early experiments included the quantitative determination of the microstructure of porous silica precursor bodies (12), which later led to a characterization of porosity over nearly three decades in length scale (13). Porous materials are used in a wide variety of engineering applications, including super insulators, membranes, catalyst supports, and porous hosts for second-phase filtration. Because microstructure and performance are strongly related, the realization of different applications depends on the ability to produce porous media with specific pore sizes and pore-size distributions. The sol-gel fabrication fabrication (fab´rikā´shn),
n the construction or making of a restoration. route has been used for many polymer-based materials schemes because of the flexibility it offers to create different microstructural products. In the study of sol-gels described here, USAXS measurements on X23A3 were complemented by electron microscopy and small-angle neutron scattering Small angle neutron scattering (SANS) is a laboratory technique, similar to the often complementary techniques of small angle X-ray scattering (SAXS) and light scattering. These are particularly useful because of the dramatic increase in forward scattering that occurs at phase measurements to quantify the microstructural features within porous silica gels. The size distributions were derived from a maximum entropy analysis of the scattering data (Fig. 4).
The materials had been prepared from 20 % mass fraction colloidal colloidal
of the nature of a colloid.
a bath containing gelatin, bran, starch or similar substances, to relieve skin irritation and pruritus. silica and 80 % mass fraction potassium silicate silicate, chemical compound containing silicon, oxygen, and one or more metals, e.g., aluminum, barium, beryllium, calcium, iron, magnesium, manganese, potassium, sodium, or zirconium. Silicates may be considered chemically as salts of the various silicic acids. . These precursor bodies are typically only 15 % to 20 % of theoretical density, and before densification, they are leached to remove the alkali content. Fig. 4 compares the microstructure of leached and unleached samples. The most striking feature in this derived size distribution is a narrow peak between 2 nm and 3 nm. This feature is evident in the results from both the unleached and the leached samples. It is attributed to nanometer-scale porosity in the leached samples and is attributed to similarly sized alkali-silicate-rich regions in the unleached samples. The increased scattering contrast of silica-to-void compared to silica-to-silicate accounts for the increased intensity in the scattering of the leached sample. At large diameters, there is a peak at nearly 55 nm, which represents the silica clusters. The unusual observation of skeletal voids within the solid phase, and solid clusters wi thin the void phase in the same material is a consequence of the extraordinary variety of microstructures in these gels.
In another USAXS study, the extraordinary sensitivity of the X23A3 USAXS instrument enabled the in situ In place. When something is "in situ," it is in its original location. observation of x-ray scattering from dislocation structures during the deformation of single crystal aluminum (14). Attempts over the years to measure small-angle scattering from dislocation structures have mostly met with limited success for various reasons. One of the earliest recognized reasons was the intrusion into the data of double-Bragg diffraction. Another problem was surface scattering from improperly prepared surfaces. Finally, unless the scattering vector is nearly perpendicular to a dislocation line, no appreciable scattering is seen. By avoiding double-Bragg diffraction conditions, meticulous sample surface preparation, and by orienting the samples for dislocation visibility, it was possible to observe: 1. correlations in the ordered fraction of dislocations, 2. the presence of dislocation dipoles, 3. the increasing dislocation content with increasing strain, and 4. the decreasing width of the interface between the dislocation walls and the surrounding, nearly-dislocation-free material. In Fig. 5, the increasing dislocation content with increasing strain can be seen directly from the slit-smeared USAXS from single-crystal aluminum at strains of 0.4 %, 0.9 %, 2.2 %, 3.6 %, 4.4 %, 5.3 %, and 6.7 %.
After 15 years of successful operation, X23A3 was closed in 2000 when the next-generation USAXS and topography instruments went into commissioning at the APS.
2.3 X-Ray Absorption Fine Structure
The X23A2 beam line provides a stable, scanning, highly monochromatic x-ray beam x-ray beam,
n the spatial distribution of radiation emerging from a radiograph generator or source. The colloquial term for radiographic beam. See radiographic beam. covering the energy range of 4.9 keV to over 30 keV. It was designed and built by scientists in the Electrical and Electronic Engineering Laboratory at NIST. In 1991, two of the scientists and the instrumentation became part of MSEL. Work performed on X23A2 has focused on bond distortions in the GeSi (15), the AlGaN (16), and the InGaAs (17, 18) alloy systems. A large fraction of this work addressed questions related to the strain and bond distortions in thin alloy films of these materials that had been grown epitaxially on substrates with dissimilar lattice constants.
X23A2 was used to develop the diffraction anomalous fine structure technique (DAFS) (19,20). All of these studies required the extremely stable, broad energy scanning capabilities of the beam line. The analysis of the XAFS and DAFS data enabled the development of a microscopic model that describes the local atomic distortions in strained films that is based on the random cluster approximation and the Keating valence force field within the context of macroscopic macroscopic /mac·ro·scop·ic/ (mak?ro-skop´ik) gross (2).
mac·ro·scop·ic or mac·ro·scop·i·cal
1. Large enough to be perceived or examined by the unaided eye.
2. elastic theory (21). Fig. 6 compares the experimental bond lengths for strained [Ga.sub.1_x][In.sub.x]As films grown on both GaAs (001) and InP (001) substrates with the theoretical predictions. The large departures of the strained bond lengths from the bond lengths in the cubic, unstrained alloys as a function of substrate lattice constant are noteworthy. Clearly, these distortions are found to oppose the natural bond-length distortions due to alloying.
More recent work using X23A2 addressed the structure of passive oxide films grown on GaAs (001) (22). It was determined that the bond length in a 23 A [Gd.sub.2][O.sub.3] film grown epitaxially on GaAs (001) was strained +2.7 %[+ or -]0.6 % relative to the bond length in bulk [Gd.sub.2][O.sub.3] powder. Using a simple model for the strained film based on the phenomenology phenomenology, modern school of philosophy founded by Edmund Husserl. Its influence extended throughout Europe and was particularly important to the early development of existentialism. developed for strained semiconductor alloys, lattice matching of the  and [-110] axes of the [Gd.sub.2][O.sub.3] film with the  and [1-10] axes of the GaAs (001) surface, the measured bond length is in excellent agreement with the perpendicular lattice constant of the film as determined by x-ray diffraction (Fig. 7).
While X23A2 provides relatively hard energy x rays, X24A offers x rays in the tender energy range of 1.7 keV to 6 keV which NIST scientists have used for x-ray standing wave, x-ray fluorescence, and x-ray photoelectron spectroscopy X-ray Photoelectron Spectroscopy (XPS) is a quantitative spectroscopic surface chemical analysis technique used to estimate the empirical formula or elemental composition, chemical state and electronic state of the elements on the surface (upto 10 nm) of a material. experiments. The facility is supported by three laboratories within NIST (MSEL, the Chemical Sciences and Technology Laboratory, and the Physics Laboratory), the NSLS, and the University of Rhode Island History
The University was first chartered as the state's agricultural school in 1888. The site of the school was originally the Oliver Watson Farm, and the original farmhouse still lies on the campus today. . In the past, the x-ray standing wave technique was used to determine the atomic-scale structure of over layer atoms on single crystal surfaces (23), of interfacial atoms in buried semiconductor interfaces (24), and of reconstructed atoms at clean semiconductor surfaces (25).
Recently, NIST researchers combined high-resolution x-ray photoelectron spectroscopy with the site-specificity of x-ray standing-wave diffraction to develop a new technique by which the partial densities of occupied electronic states of single crystals may be obtained (26). To illustrate the principle of the technique, Fig. 8 compares two x-ray photoelectron pho·to·e·lec·tron
An electron released or ejected from a substance by photoelectric effect.
photoelectron spectra from the rutile rutile, mineral, one of three forms of titanium dioxide (TiO2; see titanium). It occurs in crystals, often in twins or rosettes, and is typically brownish red, although there are black varieties. [TiO.sub.2] (110) surface recorded within the energy width of the [TiO.sub.2] (200) Bragg back-reflection condition (hv[approximately equal to] 2700 eV). The spectra extend over the kinetic-energy range of the Ti 3p, the O 2s, and the valence-electron emission. The photon energies were chosen to maximize either the electric-field intensity on the Ti atoms (bold line) or on the O atoms (shaded line). The data exhibit the well-known x-ray standing wave effect for both the Ti 3p and O 2s core lines, as well as for the crystal valence band. The resulting atomically resolved components of the crystal valence band are shown in Fig. 9. Th ese data are compared to ab initio [Latin, From the beginning; from the first act; from the inception.] An agreement is said to be "void ab initio" if it has at no time had any legal validity. local density approximation calculations of the partial density of states In statistical and condensed matter physics, Density of states (DOS) is a property that quantifies how closely packed energy levels are in a quantum-mechanical system. It is usually denoted with one of the symbols g, of rutile Ti[O.sub.2] that have been corrected for the angular-momentum-dependent photoelectron matrix elements of the Ti 4s, 4p, and 3d orbitals, as well as the O 2s and 2p orbitals (27). The agreement between theory and experiment is startling star·tle
v. star·tled, star·tling, star·tles
1. To cause to make a quick involuntary movement or start.
2. To alarm, frighten, or surprise suddenly. See Synonyms at frighten. , revealing the chemical hybridization hybridization /hy·brid·iza·tion/ (hi?brid-i-za´shun)
1. crossbreeding; the act or process of producing hybrids.
2. molecular hybridization
3. on each site that is directly responsible for the solid-state electronic structure.
2.5 Soft X-Ray Spectroscopy
The U7A soft x-ray materials characterization facility utilizes polarized A one-way direction of a signal or the molecules within a material pointing in one direction. soft x rays between 180 eV and 1500 eV to reveal the structure and chemical nature of diverse materials. U7A, which is operated as a partnership between NIST, The Dow Chemical Company The Dow Chemical Company (NYSE: DOW TYO: 4850 ) is an American multinational corporation headquartered in Midland, Michigan. Overview
The Dow Chemical Company is currently the second largest chemical manufacturer in the World (after BASF). , (#) and Brookhaven National Laboratory, achieved fully dedicated operation in 1996. The broad array of research includes model catalyst systems (28) polymer surfaces and their interfaces (29) magnetic hard disk lubricants (30), biological materials (31) and high temperature superconductors (32). Utilizing partial electron yield and fluorescence yield detection, surface ([approximately equal to]2 nm) and bulk ([approximately equal to]200 nm) structure and chemistry can be recorded simultaneously utilizing soft x-ray near-edge X-ray absorption fine structure (NEXAFS) (33).
Recently, NIST researchers, in collaboration with scientists from the North Carolina State University History
In a recent biopolymer bi·o·pol·y·mer
A macromolecule, such as a protein or nucleic acid, that is formed in a living organism.
any protein or nucleic acid produced by a living organism. application with the NIST Orthopedic Wear Consortium, the U7A beam line was used to investigate the wear properties of ultra-high molecular weight polyethylene (UHMWPE UHMWPE Ultra-High Molecular Weight Polyethylene ). Over half a million patients receive artificial joint replacements annually, and practically all the replacements consist of a sliding pair represented by a polymer (UHMWPE) and a hard counterface (metal or ceramic). For the past 30 years UHMWPE has remained the dominant polymer in artificial joints due to its outstanding properties. Nevertheless, it is now recognized that wear of UHMWPE contributes to the eventual loosening of the implants and is the main cause for the failure of long-term implants. Hence there is an urgent need to understand the mechanism and the surface morphology leading to wear and failure of the artificial joint. Current methods of inferring or deducing orientation information for UHMWPE lack surface sensitivity and mostly rely on staining the specimens followed by SEM examination. Soft-x-ray meas urements on U7A were able to indicate conclusively that on average at least 90 % or [+ or -] 5 % of the polyethylene molecular chains are preferentially aligned parallel to the rubbing direction, whereas samples that have not undergone rubbing stress yield nearly isotropic Refers to properties that do not differ no matter which direction is measured. For example, an isotropic antenna radiates almost the same power in all directions. In practice, antennas cannot be 100% isotropic. or random orientation of polyethylene chains. In addition, it was deduced that on average very few of the polyethylene molecular chains are aligned perpendicular to the rubbing direction. Thus, the molecular chain orientation of rubbed UHMWPE used in artificial joints could be determined conclusively and non-destructively.
3. NIST Programs in the UNICAT Collaboration at the Advanced Photon Source
The UNICAT (University-National Lab-Industry Collaborative Access Team) at the Advanced Photon Source--which includes NIST, the University of Illinois at Urbana/Champaign, Oak Ridge National Laboratory, and UOP--supports a broad range of research techniques. These include: ultra-small-angle x-ray scattering, high resolution x-ray diffraction, surface x-ray diffraction, diffuse x-ray scattering, x-ray topography, XAFS, magnetic scattering, and x-ray tomography. To meet the technical demands of our diverse experimental portfolio, the UNICAT beam lines on Sector 33 exploit the brilliance of the APS source to deliver x rays with high flux and with energy resolution better than or equal to the lifetime-broadened core-hole widths for all accessible K and L shells. The insertion device beam line, 33-ID, became operational November 1, 1999, and as of November 1, 2000, has entertained independent investigators as well as collaborative access team members. The bending magnet beam line, 33-BM, went into commissioning in March 2001 and is expected to become fully operational by the end of 2001.
3.1 Ultra-Small-Angle X-Ray Scattering and Imaging
Ultra-small-angle x-ray scattering (USAXS) was the first of the NIST-responsible experiments to come on line (36). It enables researchers to measure data in the usually inaccessible scattering vector, Q, range (where \Q\ = (4[pi]/[lambda]) sin[theta Theta
A measure of the rate of decline in the value of an option due to the passage of time. Theta can also be referred to as the time decay on the value of an option. If everything is held constant, then the option will lose value as time moves closer to the maturity of the option. ], [lambda] is the x-ray wavelength and 2[theta] is the scattering angle) down to nearly 1 X [10.sup.-4] [A.sup.-1]. The UNICAT instrument includes several capabilities that make it among the best in the world. It covers an unprecedented \Q\ range from 0.00012 [A.sup.-1] to 1.0 [A.sup.-1]; anomalous-USAXS can be acquired to investigate separately and quantify previously inseparable microstructures; and it supports the new technique of USAXS imaging. In addition, an optional "effective-pinhole" configuration is available in which transverse crystal reflections are added, thereby removing the intrinsic slit smearing of USAXS. In the effective pinhole geometry, the resolution of the scattering vector increments can be made exceedingly fine, easily surpassing that of true pinhole instruments with a 2D detector. The USAXS instrument presently enjoys the highest demand of any instrument on UNICAT.
In a recent UNICAT USAXS ceramic deformation study, x-ray scattering by silicon nitride was measured as a function of tensile strain in an effort to improve the understanding of the mechanisms controlling creep. In an attempt to improve creep resistance, which ultimately limits the lifetime of ceramic [Si.sub.3][N.sub.4] components, rare-earth-based secondary phases have been added. In this study, two commercial silicon nitride formulations were measured, including a new one that exhibits an increase in creep resistance of more than three orders of magnitude and an increase in lifetime of over two orders of magnitude. To understand the reasons for such a dramatic improvement in creep resistance, anomalous USAXS data were recorded to measure both the secondary (additive) phase and the porous phase as a function of tensile deformation. Ordinarily, scattering from the large volume fraction (from approximately 5 % to 10 %) of secondary phase would dominate the scattering from the creep void fraction (0 % to 2.5 % ), and an analysis of creep cavities could not be done. By means of anomalous scattering measurements and analysis, such quantification is rigorously possible (37). The USAXS results indicated that in the new formulation of silicon nitride, cavitation cavitation
Formation of vapour bubbles within a liquid at low-pressure regions that occur in places where the liquid has been accelerated to high velocities, as in the operation of centrifugal pumps, water turbines, and marine propellers. does not occur, compared to the other grade of [Si.sub.3][N.sub.4]. Fig. 11 shows the contribution of cavities to tensile strain in the new SN281 compared to the older SN88. Redistribution of the secondary phases via grain boundary sliding and solution-precipitation may serve as the creep mechanism.
Another example of UNICAT USAXS studies involved the characterization of the nature of the amorphous calcium-silicate-hydrate (C-S-H) gel that is the main strength-giving phase in hydrating cementitious ce·men·ti·tious
Of or relating to a chemical precipitate, especially of carbonates, having the characteristics of cement.
[From Latin caement systems including concrete. Here, the ability of the USAXS instrument to provide a primary absolute calibration of the scattered intensity with respect to the incident beam (without the need for a secondary scattering standard) proves critical. Absolute-calibrated USAXS and small-angle neutron scattering (SANS) contrast variation studies were combined in a study to determine, as independently as possible, the formula and density of the C-S-H solid phase that could be compared with various previously proposed models for C-S-H (38)). Fig. 12 shows an absolute comparison of USAXS and SANS data for a 28 day old ordinary Portland cement as a function of Q. The USAXS data were corrected for multiple scattering effects observed at low Q and the most affected data, for Q <0.0005 [A.sup.-1] were discarded. Figure 12 shows that the fractal C-S-H gel structure observed by USAXS extends to significantly lower Q (and correspondingly higher scale-lengths) observed in the SANS range. The ratio of USAXS to SANS calibrated cal·i·brate
tr.v. cal·i·brat·ed, cal·i·brat·ing, cal·i·brates
1. To check, adjust, or determine by comparison with a standard (the graduations of a quantitative measuring instrument): intensities at high Q (most sensitive to the C-S-H:[H.sub.2]O interface), when combined with other information, is found consistent with only one of the models for solid C-S-H previously proposed. Apart from solving this problem these studies also resolved a discrepancy between absolute-calibrated SANS and earlier SAXS SAXS Small Angle X-Ray Scattering determinations of the C-S-H:[H.sub.2]O interfacial surface area. The earlier SAXS studies had not been absolute-calibrated but relied on an integrated scattering approach (the "scattering invariant (programming) invariant - A rule, such as the ordering of an ordered list or heap, that applies throughout the life of a data structure or procedure. Each change to the data structure must maintain the correctness of the invariant. " method) and had yielded surface-area values two to six times higher than the SANS values. In the present study these discrepancies could be traced to uncertainties in the interpolation interpolation
In mathematics, estimation of a value between two known data points. A simple example is calculating the mean (see mean, median, and mode) of two population counts made 10 years apart to estimate the population in the fifth year. and normalization In relational database management, a process that breaks down data into record groups for efficient processing. There are six stages. By the third stage (third normal form), data are identified only by the key field in their record. of data required in the scattering invariant method, and the absolute-calibrated USAXS and SANS surface areas were found to be completely consistent.
The ultra-small-angle scattering curve and its transform lead directly to the volume-averaged determination of many microstructural parameters. However, USAXS cannot measure the homogeneity or lack thereof in a sample, and one must usually rely on complementary techniques for information on the distribution of microstructures and their morphology. In response to the need for this kind of microstructural information, as well as the need to quantify it, NIST researchers are developing the new technique of USAXS imaging (39). In this application, the UNICAT USAXS instrument is used with a 2-reflection collimator collimator (kol´imātur),
n a diaphragm or system of diaphragms made of an absorbent material and designed to define the dimensions and direction of a beam of radiation. before the sample and a 2-reflection analyzer after the sample. With the analyzer crystal pair set to \Q\ equals zero, and the photodiode A light sensor (photodetector) that allows current to flow in one direction from one side to the other when it absorbs photons (light). The more light, the more the current. Used to detect light pulses in optical fibers and other light-sensitive applications, it works the opposite of a detector replaced by an imager, a high-resolution radiograph radiograph /ra·dio·graph/ (-graf?) the film produced by radiography.
n. of the sample can be obtained. With the analyzer set to an angle within its rocking curve, a diffraction-enhanced image (which is a form of "phase contrast imaging") is obtained. Finally, with the analyzer cr ystal set to an angle within the small angle scattering regime, USAXS images are obtained. The photons that produce the image have scattered from the internal density fluctuations in and on the sample (at intensities [approximately equal to][10.sup.-2] to [10.sup.-8] of maximum). This is possible only at angles where the scattered intensity exceeds the transmitted intensity (well away from the transmitted beam). In this manner, the microstructures contributing to the scattering at that particular angle-filtered window, [DELTA]Q, are imaged. By using images created at different scattering vectors, it is possible under certain conditions to view different-sized features within a single volume. By rotating the sample about a single scattering vector, stereo pairs can be produced, and 3D information is gained. Finally, even when USAXS imaging is not used for three-dimensional imaging purposes, it is a useful adjunct to USAXS in that it offers a means of identifying spurious effects such as double Bragg diffractio n and surface scattering, and the opportunity to avoid them. Although metallic, ceramic, polymer and biological structures have been imaged, the emphasis of USAXS imaging research has mostly been on creep cavitation and ductile fracture in metals. In a recent study, ductile fracture of pure copper was investigated. Fig. 13 shows images taken close to and distant from a crack. The microstructures that are imaged are creep cavities that have formed at the grain boundaries. The data show that the microstructures far from the crack are similar in quality from those near the crack, but very different in quantity.
3.2 Looking Toward the Future at the Advanced Photon Source
At the time of this writing, two additional NIST-responsible instruments are being commissioned: x-ray topography and x-ray absorption fine structure. A third, x-ray microtomography, is still under development. Just over the horizon, NIST and UOP LLC are contemplating the possibility of joining the University of Illinois and Oak Ridge National Laboratory in the commissioning, operation and utilization of the microbeam capability of Sector 34.
In 1984, NIST's synchrotron facilities were inaugurated with the commissioning of a single beam station at the NSLS for x-ray topography. Today, the combined portfolio of NIST/MSEL facilities with our partners at the NSLS and with UNICAT at the APS offers measurement capabilities in ultra-small-angle x-ray scattering, high-resolution x-ray topography, hard and soft XAFS, and standing-wave x-ray diffraction. It also offers access to leading edge instruments for structural crystallography and time-resolved structural scattering, surface and interface scattering, diffuse scattering and magnetic scattering. The NIST synchrotron facilities enable researchers to use these intense x-ray sources for the advancement of science and technology in materials, physics, chemistry, and, most recently, biology. The primary thrust is the application of leading-edge x-ray scattering and imaging to a broad range of scientific problems and the continued development of novel techniques for innovative research. MSEL welcomes use of its synchrotron-based facilities by researchers at NIST and from other National Laboratories, universities, and industry.
[FIGURE 4 OMITTED]
[FIGURE 5 OMITTED]
[FIGURE 6 OMITTED]
[FIGURE 8 OMITTED]
[FIGURE 9 OMITTED]
[FIGURE 10 OMITTED]
[FIGURE 11 OMITTED]
[FIGURE 12 OMITTED]
We note the many contributions of our wonderful colleagues and collaborators that were instrumental to the success of the MSEL endeavor. In particular, we mention Masao Kuriyama, Bill Boettinger, Ron Dobbyn, Bruce Steiner, Chuck Bouldin, Richard Deslattes, Paul Cowan, Terry Jach, Ben DeKoven, Sara Sambasivan, Timm Richardson, Zugen Fu, Steve Hulbert at the NSLS, and Pete Jemian, Jan Ilavsky, Jenia Karapetrova, Paul Zschack, Gene Ice, Hawoong Hong, and Haydn Chen at the APS for their key efforts leading to the remarkable capabilities of these facilities.
The X23A2 facility at the NSLS is supported by NIST [U.S. Department of Commerce (DoC)]. X24A is supported by three laboratories within NIST (MSEL, the Chemical Sciences and Technology Laboratory, and the Physics Laboratory), the NSLS, and the University of Rhode Island. U7A is supported by NIST, Dow, and Brookhaven National Laboratory (DoE). Use of the NSLS is supported by the U.S. Department of Energy (DoE) under contract no. DE-AC02-98CH10886.
The UNICAT facility at the APS is supported by the University of Illinois at Urbana/Champaign, Materials Research Laboratory (U.S. Department of Energy (DoE), the State of Illinois (IBHE-HECA) and the U.S. National Science Foundation), Oak Ridge National Laboratory (U.S. DoE), NIST (U.S. DoC), and UOP LLC. Use of the APS is supported by the U.S. DoE, Basic Energy Sciences, Office of Science, under contract no. W-31-109-ENG-38.
Accepted: August 22, 2001
Available online: http://www.nist.gov/jres
(#.) Certain commercial equipment, instruments, or materials are identified in this paper to foster understanding. Such identification does not imply recommendation or endorsement by the National Institute of Standards and Technology, nor does it imply that the materials or equipment identified are necessarily the best available for the purpose.
(1.) M. Kuriyama, W. J. Boettinger, and G. G. Cohen cohen
(Hebrew: “priest”) Jewish priest descended from Zadok (a descendant of Aaron), priest at the First Temple of Jerusalem. The biblical priesthood was hereditary and male. , Synchrotron radiation topography, in Ann. Rev. Mater. Sci. 12, 23-50 (1982).
(2.) M. Kuriyama, R. C. Dobbyn, R. D. Spal, H. E. Burdette, and D. R. Black, Hard x-ray microscope x-ray microscope
An instrument using x-rays to render a highly magnified image. with submicrometer spatial resolution (Data West Research Agency definition: see GIS glossary.) A measure of the accuracy or detail of a graphic display, expressed as dots per inch, pixels per line, lines per millimeter, etc. It is a measure of how fine an image is, usually expressed in dots per inch (dpi). , J. Res. Natl. Inst. Stand. Technol. 95, 559-574 (1990).
(3.) G. G. Long, P. R. Jemian, and J. R. Weertman, High-resolution small-angle x-ray-scattering camera for anomalous scattering, J. Appl. Crystallog. 24, 30-37 (1991).
(4.) A. J. Allen, S. Krueger, G. Skandan, G. G. Long, H. Hahn, H. M. Kerch, J. C. Parker, and M. N. Ali, Microstructural evolution during the sintering sintering, process of forming objects from a metal powder by heating the powder at a temperature below its melting point. In the production of small metal objects it is often not practical to cast them. of nanostructured ceramic oxides, J. Amer. Ceram. Soc. 79, 1201-1212 (1996).
(5.) P. R. Jemian, J. R. Weertman, G. G. Long, and R. D. Spal, Characterization of 9Cr-1MoVNb steel by anomalous small angle x-ray scattering, Acta Metallurg. Mater. 39, 2477-2487 (1991).
(6.) B. J. Olivier, R. R. Lagasse, D. W. Schaefer, J. D. Barnes, and G. G. Long, A small-angle scattering study of pore orientation periodicity periodicity /pe·ri·o·dic·i·ty/ (per?e-ah-dis´i-te) recurrence at regular intervals of time.
1. in porous polymer and carbon structures, Macromolecules Macromolecules
A large molecule composed of thousands of atoms.
Mentioned in: Gene Therapy
macromolecules 29, 8615-8621 (1996).
(7.) S. Krueger, G. J. Olson, D. Johnsonbaugh, and T. J. Beveridge, Characterization of the binding of gallium, platinum and uranium to Pseudomonas Fluorescens by small-angle x-ray scattering Small-angle X-ray scattering (SAXS) is a small-angle scattering (SAS) technique where the elastic scattering of X-rays (wavelength 0.1 ... 0.2 nm) by a sample which has inhomogeneities in the nm-range, is recorded at very low angles (typically 0.1 - 10°). and transmission electron microscopy “TEM” redirects here. For other uses, see TEM (disambiguation).
Transmission electron microscopy (TEM) is an imaging technique whereby a beam of electrons is transmitted through a specimen, then an image is formed, magnified and directed to appear either , Appl. Environ. Microbiol. 59, 4056-4064 (1993).
(8.) W. J. Boettinger, H. E. Burdette, M. Kuriyama, and R. E. Green, Jr., Asymmetric crystal topographic camera, Rev. Sci. Instrum. 47, 906-911 (1976).
(9.) B. Steiner, U. Laor, M. Kuriyama, G. G. Long and R. C. Dobbyn. Diffraction imaging of high quality bismuth bismuth (bĭz`məth) [Ger. Weisse Masse=white mass], metallic chemical element; symbol Bi; at. no. 83; at. wt. 208.9804; m.p. 271.3°C;; b.p. about 1,560°C;; sp. gr. 9.75 at 20°C;; valence +3 or +5. silicon oxide with monochromatic synchrotron radiation: implications for crystal growth, J. Cryst. Grow. 87, 79-100 (1988).
(10.) D. Black, T. Gallagher, and L. Arnowitz, Applying x-ray topography and diffractometry to improve protein crystal growth, in Proceedings of Space Technology and Applications International Forum--2000, AIP AIP acute intermittent porphyria.
AIP Acute intermittent porphyria Conf. Proc. Vol. 504, M. S. El-Genk, ed., American Institute of Physics The American Institute of Physics (AIP) is a professional body representing American physicists and publishing physics related journals. It was founded in 1931.
The aims of the organization are: "promoting the advancement and diffusion of the knowledge of physics and its , New York New York, state, United States
New York, Middle Atlantic state of the United States. It is bordered by Vermont, Massachusetts, Connecticut, and the Atlantic Ocean (E), New Jersey and Pennsylvania (S), Lakes Erie and Ontario and the Canadian province of (2000) pp. 50-56.
(11.) A. J. Allen, P. R. Jemian, D. R. Black, H. E. Burdette, R. D. Spal, S. Krueger, and G. G. Long, Ultra-small-angle x-ray scattering to bridge the gap between visible light scattering and standard small-angle scattering cameras, Nucl. Instrum. Meth. Phys. Res. A347, 487-490 (1994).
(12.) G. G. Long, S. Krueger, P. R. Jemian, D. R. Black, H. E. Burdette, J. P. Cline, and R. A. Gerhardt, Small-angle-scattering determination of the microstructure of porous silica precursor bodies, J. App. Crystallog. 23, 535-544 (1990).
(13.) H. M. Kerch, G. G. Long, S. Krueger, A. J. Allen, R. Gerhardt, and F. Cosandey, Characterization of porosity over many length scales: Application to colloidal silica, J. Mater. Res. 14, 1444-1454 (1999).
(14.) G. G. Long, L. E. Levine, and R. Thomson, In-situ observation of small-angle x-ray scattering by dislocations, J. Appl. Crystallog. 33, 456-460 (2000).
(15.) J. C. Woicik, C. E. Bouldin, M. I. Bell, J. O. Cross, D. J. Tweet, B. D. Swanson, T. M. Zhang, L. B. Sorensen, C. A. King, J. L. Hoyt, P. Pianetta, and J. F. Gibbons Famous people named Gibbons include:
(16.) K. E. Miyano, J. C. Woicik, L. H. Robins, C. E. Bouldin, and D. K. Wickenden, Extended x-ray absorption fine structure study of [Al.sub.x][Ga.sub.1-x]N films, Appl. Phys. Lett. 70, 2108-2110, (1997).
(17.) J. C. Woicik, J. G. Pellegrino, B. Steiner, K. E. Miyano, S. G. Bompadre, L. B. Sorensen, T.-L. Lee, and S. Khalid, Bond-length distortions in strained-semiconductor alloys, Phys. Rev. Lett.79, 5026-5029 (1997).
(18.) J. C. Woicik, J. A. Gupta, S. P. Watkins, and E. D. Crozier crozier
see crosier. , Bond-length strain in buried [Ga.sub.1-x][In.sub.x]As thin-alloy films grown coherently on InP (001), Appl. Phys. Lett. 73, 1269-1271 (1998).
(19.) H. Stragier, J. O. Cross, J. J. Rehr, L. B. Sorensen, C. E. Bouldin, and J. C. Woicik, Diffraction anomalous fine structure: A new x-ray structural technique, Phys. Rev. Lett. 69, 3064-3067 (1992).
(20.) J. C. Woicik, J. O. Cross, C. E. Bouldin, B. Ravel, J. G. Pellegrino, B. Steiner, S. G. Bompadre, L. B. Sorensen, K. E. Miyano, and J. P. Kirkland, Diffraction anomalous fine structure study of strained [Ga.sub.1-x][In.sub.x]As on GaAs (001), Phys. Rev. B58, R4215-R4218 (1998).
(21.) J. C. Woicik, Random-cluster calculation of bond lengths in strained-semiconductor alloys, Phys. Rev. B57, 6266-6269 (1998).
(22.) E. J. Nelson, J. C. Woicik, M. Hong, J. Kwo and J. P. Mannaerts, Extended x-ray absorptions fine structure measurements of bond-length strain in epitaxial [Gd.sub.2][O.sub.3] on GaAs (001) Applied Phys. Lett. 76, 2526-2528 (2000).
(23.) J. C. Woicik, T. Kendelewicz, K. E. Miyano, P. L. Cowan, C. E. Bouldin, B. A. Karlin, P. Pianetta, and W. E. Spicer, Determination of the Sb/Si (111) interfacial structure by back reflection x-ray standing wave and surface extended x-ray absorption fine structure techniques, Phys. Rev. B44, 3475-3478 (1991).
(24.) J. C. Woicik, J. G. Pellegrino, S. H. Southworth, P. S. Shaw, B. A. Karlin, C. E. Bouldin, and K. E. Miyano, Accommodation of strain in ultra-thin InAs/GaAs films, Phys. Rev. B52, R2281-R2284 (1995).
(25.) J. C. Woicik, T. Kendelewicz, K. E. Miyano, P. L. Cowan, C. E. Bouldin, B. A. Karlin, P. Pianetta, and W E. Spicer, X-ray standing wave determination of the clean InP (110) surface reconstruction, Phys. Rev. Lett. 68, 341-344 (1992).
(26.) J. C. Woicik, E. J. Nelson, D. Heskett, J. Warner, L. E. Berman, B. A. Karlin, I. A. Vartanyants, M. Z. Hasan, T. Kendelewicz, Z. X. Shen Shen, in the Bible, place, perhaps close to Bethel, near which Samuel set up the stone Ebenezer. , and P. Pianetta, X-ray standing-wave investigations of valence-electronic structure, Phys. Rev. B64, 125115 (2001).
(27.) J. C. Woicik, E .J. Nelson, L. Kronik, M. Jain, J. R. Chelikowsky, D. Heskett, L. E. Berman, and G. S. Herman, Direct experimental observation of chemical hybridization in rutile [TiO.sub.2] using site-specific x-ray photoelectron spectroscopy, submitted for publication, Phys. Rev. Lett. (2001).
(28.) A. Kuperman, S. Sambasivan, D. A. Fischer, and B. M. DeKoven, Direct observation of propylene propylene /pro·pyl·ene/ (pro´pi-len) a gaseous hydrocarbon, CH3CHdbondCH2.
propylene glycol a colorless viscous liquid used as a humectant and solvent in pharmaceutical preparations. transformation on chemistry and in the pores of silver exchanged faujasite catalyst, Adv. Mater. 12,1809-1813 (2000).
(29.) D. L. Schmidt, C. E. Coburn, B. M. DeKoven, G. E. Potter, G. F. Meyers, and D. A. Fischer, A water-based, non-stick, hydrophobic hydrophobic /hy·dro·pho·bic/ (-fo´bik)
1. pertaining to hydrophobia (rabies).
2. not readily absorbing water, or being adversely affected by water.
3. coating system, Nature 368, 39-41 (1994).
(30.) H. J. Kang, Q. Zhao, F. E. Talke, D. J. Perettie, B. M. DeKoven, T. A. Morgan, D. A. Fischer, S. M. Hsu, and S. Bhatia, The use of cyclic phosphazine additives to enhance the performance of the head/disk interface, Lubricat. Eng. 55, 22-27 (1999).
(31.) D. A. Fischer, S. Sambasivan, M. Shen, and S. M. Hsu, Wear induced molecular orientation in ultra-high-molecular-weight polyethylene (UHMWPE); the effect of surface energy and orientation, Trans. Soc. Biomater., 22, 352-(1999).
(32.) A. R. Moodenbaugh, B. Nielsen, S. Sambasivan, D. A. Fischer, T. Friessnegg, S. Aggarwal, R. Ramesh, and R. L. Pfeffer, Hole-state density of [La.sub.1-x][Sr.sub.x]Co[O.sub.3-[delta]] (0 [less than or equal to] X [less than or equal to] 0.5) across the insulator/metal phase boundary, Phys. Rev. B61, 5666-5671 (2000).
(33.) D. A. Fischer, G. E. Mitchell, B. M. DeKoven, A. T. Yeh, J. L. Gland, and A. R. Moodenbaugh, Ultra-soft x-ray absorption spectroscopy The X-ray absorption spectroscopy is currently a widely used technique giving information on the local structure and on the electronic states in gas-phase, molecular and condensed matter. : a bulk and surface probe of materials, in Applications of Synchrotron Techniques to Materials Science, MRS MRS - Modifiable Representation System.
An integration of logic programming into Lisp.
["A Modifiable Representation System", M. Genesereth et al, HPP 80-22, CS Dept Stanford U 1980]. Symp. Proc. Vol. 307, Applications of Synchrotron Radiation Techniques to Materials Science, D. Perry, R. Stockbauer, N. Shinn, K. D'Amico, and L. Terminello, eds., Materials Research Society, Pittsburgh (1993) pp. 101-106.
(34.) W. E. Wallace, D. A. Fischer, K. Efimenko, W. L. Wu, and J. Genzer, Polymer chain relaxation: surface outpaces bulk, Macromolecules 34, 508 1-5082 (2001).
(35.) P. G. deGennes, Glass transitions in thin polymer films, Europ. Phys. J. 2, 201-205 (2000).
(36.) G. G. Long, A. J. Allen, J. Ilavsky, P. R. Jemian, and P. Zschack, The ultra-small-angle x-ray scattering instrument on UNICAT at the Advanced Photon Source, in American Institute of Physics Conf. Proc. 521, Synchrotron Radiation Instrumentation: 11th U.S. National Conference, P. Pianetta, J. Arthur, and S. Brennan, eds., American Institute of Physics, Melville, NY (2000) pp. 183-187.
(37.) P. R. Jemian, G. G. Long, F Lofaj, and S. M. Wiederhorn, Anomalous ultra-small-angle x-ray scattering from evolving microstructures during creep, in plications of Synchrotron Radiation Techniques to Materials Science V, MRS Conf. Proc. Vol.590,S. R. Stock, S. M. Mini, and D. L. Perry, eds., Materials Research Society, Warrensdale, PA (2000) pp. 131-136.
(38.) J. J. Thomas, H. M. Jennings, and A. J. Allen, The Surface of Hardened Cement Paste as Measured by Various Techniques, Concrete Sci. Eng. 1, 45-64 (1999).
(39.) G. G. Long, L. E. Levine, and R. J. Fields, X-ray scattering and imaging from plastically deformed metals, Mater. Sd. Eng. A309-A310, 28-31 (2001).
About the authors: All of the authors are members of the Materials Microstructure Characterization Group in the Ceramics Division of the NIST Materials Science and Engineering Laboratory. Gabrielle Long is Leader of the Group. Her research interests include materials microstructure, materials deformation, x-ray and neutron scattering and x-ray imaging. Andrew Allen's research interests include experimental studies of the microstructures of ceramic coatings, cements and nanomaterials, and the application of neutron scattering to anisotropic Refers to properties that differ based on the direction that is measured. For example, an anisotropic antenna is a directional antenna; the power level is not the same in all directions. Contrast with isotropic. materials. David Black's research interests include crystal perfection studied by means of x-ray topography and the study of low-Z materials using inelastic inelastic
Of or relating to the demand for a good or service when quantity purchased varies little in response to price changes in the good or service. x-ray scattering. Harold Burdette areas of specialization include x-ray optical instrumentation and materials characterization. Daniel Fischer is Spokesperson for the U7A beam line at the NSLS, and his area of specialization is materials characterization through the development and application of in situ synchrotron rad iation spectroscopies via novel detection methods. Richard Spal's research interests include x-ray microscopic investigation of superconductor A material that has little resistance to the flow of electricity. Traditional superconductors operate at absolute zero (-459.67 degrees Fahrenheit or -273.15 degrees Celsius). Experiments in the 1980s raised the temperature to -321 degrees Fahrenheit. structures and other materials. Joseph Woicik is Spokesperson for the X23A2 beam line at the NSLS and his research interests include atomic-level structures at semiconductor surfaces and interfaces, and the site-specific electronic structures of materials. The National Institute of Standards and Technology is an agency of the Technology Administration, U.S. Department of Commerce.